International Journal of Engineering and Technical Research (IJETR) ISSN: 2321-0869, Volume-2, Issue-10, October 2014
Microstructural and photo-induced properties of silver-doped in situ crystallized TiO2 coatings prepared by reactive magnetron sputtering I. Sayah, M. Arab Pour Yazdi, F. Schuster, A. Aouni and A. Billard Abstract- The aim of this study is to investigate the influence of in-situ crystallization on the microstructural and the photocatalytic properties of silver doped TiO2 coatings deposited on glass slides at different temperatures. Then, a first step of this work consisted in depositing a SiNx barrier layer on the glass slide to prohibit further diffusion of alkali elements and poisoning of the active layer. The second step was to synthesize pure TiO2 and silver-doped TiO2 films at high pressure by magnetron sputtering at the 400°C. Silver was introduced in the coatings at different contents by co-sputtering simultaneously of titanium and silver target. The samples were characterized by X-ray diffraction, scanning electron microscopy and finally the photocatalytic activity was assessed by using the Orange G decomposition upon UV or visible irradiations. Index Terms—Photocatalysis-titanium dioxide-magnetron sputtering-silver doped Titania.
I. INTRODUCTION In order to solve environmental problems relating to wastewaters, TiO2 photocatalyst has been intensively studied due to its ability to degrade a wide range of organic pollutants, its physical and chemical stability, low-cost and non-toxicity . Photocatalysis is a catalytic oxidation process involving a solid photocatalyst and ultraviolet radiation. It appears as one of cheaper processes, which has been established for conducting the degradation of organic molecules in aqueous or gas phase. It’s a process that involves the occurrence of a chemical reaction in the presence of semiconductor TiO2 irradiated with energy higher than its band gap . The electrons e- are excited from the valence band into the conduction band leaving holes h+ in the valence band. Such activated electrons or holes can diffuse to the surface and generate different types of radicals or ions which are highly reactive with contacting organic compounds adsorbed on the
Manuscript received October 22, 2014. Sayah, IRTES-LERMPS, UTBM, site de Montbéliard, 90010 BELFORT CEDEX, FRANCE. LMVR, FSTT, Tangier, Morocco M. Arab Pour Yazdi, IRTES-LERMPS, UTBM, site de Montbéliard, 90010 BELFORT CEDEX, FRANCE F. Schuster, CEA/ Cross-cutting program on advanced materials. LRC CEA/IRTES-LERMPS. A. Aouni, LMVR, FST de Tanger, Maroc A. Billard, LRC CEA/IRTES-LERMPS
titania surface and can decompose them . Many methods can be used to prepare TiO2 films include sol-gel method , chemical vapour deposition , sputtering process , vacuum evaporation , ion beam techniques , filtered arc deposition . Among them the magnetron sputtering presents numerous advantages especially the high quality and homogeneity of obtained films, large-area of uniform coatings and strong adhesion. Furthermore, magnetron sputtering provides more advantages in controlling the microstructure, the morphology and hence the properties of the titania films by modifying the deposition parameters such as the working pressure, the oxygen-partial pressure, the draw distance and the substrate temperature. However, TiO2 has a relatively high bandgap (Eg > 3.2 eV) and can only excited by UV irradiation. In order to make it work under visible light irradiation, many studies proposed doping of TiO2 with some transition metals . Among these metals especially silver, have received much attention for this purpose . In this work, we have investigated the structural and photocatalytic properties of undoped and silver doped TiO2 coatings deposited on glass slides at high pressure and temperature. II. EXPERIMENTAL DETAILS Undoped and Ag doped TiO2 films were deposited at 5 Pa by reactive DC magnetron sputtering using two metallic targets of Ti and single target of Ag of 50 mm diameter and 99.99% purity on glass slides substrates (75 × 25 mm2). The substrates are covered in the first step by 350 nm SiNx barrier layer to avoid alkali elements diffusion of glass and degradation of TiO2 photocatalytic activity . The experimental device is a 90-litre sputtering chamber pumped down via a turbomolecular pump system allowing a base vacuum of less than 10− 4 Pa. The substrate-holder was heated at 400 °C by radiative effect using an electrical resistance placed behind of the substrate-holder at about 5 mm. The details of the reactive magnetron sputtering reactor are available elsewhere . The distance between the targets and substrate holder was fixed at about 60 mm and the substrate holder was rotated regularly during the deposition run (60 RPM). In all experiments, the discharge current applied to Ti targets was fixed at 0.8 A. To obtain Ag-doped TiO2 samples with different silver ratios, Ag element was introduced in the coatings at different contents by adjusting the discharge current applied on Ag target from 5 to 8 mA. The main deposition parameters are summarized in Table 1.
Microstructural and photo-induced properties of silver-doped in situ crystallized TiO2 coatings prepared by reactive magnetron sputtering
Table1. Sputtering parameters for synthesis of undoped and Ag doped TiO2 coatings. Ar flow rate (sccm) Oxygen flow rate (sccm) Total pressure (Pa) Run duration (h) Draw distance (mm)
220 10 5 2 60
Target (metallic) Discharge current (A) Pulse frequency (kHz) Substrate temperature (°C)
Ti 0.8 50 400
Ag 0.0050.008 -
The structure of the films was characterized by X-ray diffraction in the Bragg-Brentano (θ/2θ) geometry using Bruker D8 focus diffractometer equipped with a cobalt anode (CoKα1+α2radiations). The morphology of the coatings is assessed by means of scanning electron microscopy (SEM) using a JEOL JSM 7800F equipped with energy dispersive spectroscopy (EDS) for chemical composition measurements. The photocatalytic activity was evaluated by following in real-time the Orange G decomposition (100 ml) during 2 h with an initial concentration C0 = 10 mg.l-1 upon UV irradiation from a UV–vis xenon light source (Lot-Oriel) emitting with a constant irradiance (15 mW. m-2). The distance between the samples and the light source was fixed at 15 cm. The experimental setup is described elsewhere in details . Since the degradation reaction is a pseudo one-order kinetic, the photocatalytic activity is expressed in terms of the apparent rate constant K' in min− 1.
Fig 1. X-ray diffractograms of Ag-doped TiO2 coatings in-situ annealed at 400°C. Fig 2 shows the SEM top surface views of the coatings. It can be seen clearly that the undoped TiO2 films exhibits a large porous morphology Fig (2(a)).
The photo-induced hydrophilic character of the films was studied by measuring the contact angle of constant volume water droplets deposited in ambient air on the coatings surface using DIGITROP device type after different irradiation times. The angle measurement was performed in ambient air and each angle value is an average of about five measurements on the entire coating surface. III. RESULTS AND DISCUSSION A. Structural and morphological characterization TiO2 layers enriched in different percentages of silver were analyzed by X-ray diffraction (Fig 1). Indexing of the diffraction peaks was carried from the 01-089-4921-JCPDS and 01-087-0720-JCPDS card number. TiO2 crystallizes in the anatase phase with a preferred orientation along the plane (101) and along (004) for undoped TiO2 and neither traces of parasitic phase were detected in the films. The presence of metallic Ag is visible even for Ag content as low as 1 at/.% and the Ag crystallizes in the FCC structure. By increasing the silver content, the intensity of all peaks increases, which leads to the conclusion that the particles of Ag and TiO2 grains grow gradually. For low percentages (1 and 2 at.% ), silver is dispersed in the matrix of TiO2. For larger percentages (7 and 10 at.% ), the silver particles precipitate onto the surface of the coatings and TiO2 crystallizes more coarsely in its anatase structure.
Fig 2.Top surface SEM micrographs of the surface of the synthesized TiO2 with various percentages of Ag: a): 0 at.%; b): 1 at.%; c): 2 at.% ; d): 7 at.% and e): 10 at.%.
International Journal of Engineering and Technical Research (IJETR) ISSN: 2321-0869, Volume-2, Issue-10, October 2014 The layers formed with low percentages of Ag (Fig 2 (b) and (c)) show a homogeneous and granular surface with no Ag traceless. By increasing the percentage of Ag, the Ag particles begin to agglomerate on the surface (Fig 2 (d) and (e)). These observations confirm the results obtained by the X-ray diffractograms. B. Photocatalytic properties The evolution of the apparent rate constant K’ as a function of silver content is compared for the films deposited at 400 °C under UV irradiation and visible light (Fig 3). Under UV irradiation, the apparent constant K’ of TiO2 is about 2.10-3 .min-1. It increases to 2.5 10-3 min.-1 for about 1 at.% Ag and falls to 0.7.10-3 min-1 for Ag contents higher than 7 at.%. Under visible light, it was found that as pure TiO2 is not active under visible light, increasing Ag content increases quite linearly K’ up to 1.2.10-3 min-1 for about 7 at.% Ag and then decreases K’ for higher Ag contents. Above the optimum content, the Ag particles begin to act as recombination centers thereby reducing the photocatalytic activity of the layers. Similar behavior was also observed for TiO2 layers doped FeIII, ZnII and LaIII [13-16]. Previous research of the effect of addition of Zn and Fe  has shown that even if the profile was similar to the variation, the optimal concentration varies with the nature of the metal ions used. In general, comparing the optimum content of the silver ions with FeIII of ZnII and it was found that the optimum content for the silver ions is considerably lower than that of FeIII and ZnII. This difference could be related to the degree of oxidation and the ionic radius of different metal ions. For a similar TiIV ionic radius (61 pm), FeIII (55 pm) and ZnII (74 pm) ions could enter the TiO2 lattice by substituting TiIV in the lattice sites [15-17]. In addition, they may also exist as ions in the pore network of TiO2. However, it is impossible for Ag ions whose ionic radius equal to 115 pm to act as interstitial ions in the matrix of TiO2. The silver ion can only replace TiIV in lattice sites like solid solution . Without adding another element to titanium oxide in its production, the oxygen is the only electron acceptor. However when the addition of Ag, two additional acceptor species are introduced: Ag+ and Ag. The most important advantage of adding Ag is to improve the efficiency of charge separation which increases the lifetime of the charge carriers. Thus, a greater number of holes reach the interfacial region of the layer, leading to the production of super-active groups such as: HO2•, OH• and H2O2 . The high photoactivity of TiO2 enriched Ag compared to that of pure TiO2 under UV irradiation is attributed to the fact that silver acts as an electron trap in the surface layers. This speeds up the rate of electrons transfer to molecular oxygen, inhibiting thereby the recombination of photogenerated electrons and holes .
Fig 3. Evolution of the apparent rate constant K’ as a function of Ag at.% for the coatings synthesized at 400°C. The hydrophilicity of films which have the highest photocatalytic activity was investigated by measurements of the water contact angle. Fig 4 shows the changes in this angles induced by UV light irradiation for different times (0, 15, 30, 60 and 120 min).
Fig 4. Contact angle evolution of of 7 at.% Ag doped TiO2 according to the irradiation time. The contact angle decreases with increasing the irradiation time to a value equal to 5 ° for 2 h after irradiation. This was explained by the fact that the UV-light-induced hydrophilicity of the TiO2 is related to the dissociative adsorption of water molecules from the ambient air at Ti4+ photo-reduced to Ti3+, which is typically situated at the oxygen bridges on the surface [21- 22]. IV. CONCLUSION The efficiency of undoped and Ag doped porous TiO2 thin films deposited by reactive magnetron sputtering at high pressure on heated glass slides substrates at 400 °C) was investigated. XRD analysis reveals that all the films crystallized only in the anatase structure. The morphology of the layers is porous. Under visible light, the photocatalysis processes show that 7 at.% Ag-doped TiO2 thin film is attractive for photocatalytic applications. Under UV irradiation, however, the 1 at.% Ag doped TiO2 films revealed 25% more Orange photodegradation as compared to the undoped TiO2. Finally, the hydrophilicity of films which have the highest photocatalytic activity was verified.
Microstructural and photo-induced properties of silver-doped in situ crystallized TiO2 coatings prepared by reactive magnetron sputtering REFERENCES K. Nakata, A. Fujishima, “TiO2 photocatalysis : design and applications” J. Photochem. Photobiol C. Photochem, (2012) pp: 169-198.  A. Fujishima, K. Honda, Nature 238 (1972), 37  B. Kraeutler, A.J. Bard , “ Heterogeneous photocatalytic synthesis of methane from acetic acid-new Kolbe reaction pathway”J. Am. Chem. Soc. 100 (1978), pp: 2239-2240  D. Lee, M.R. Rubner, R.E. Cohen, “All-Nanoparticle thin Film Coatings” Nano Lett. 6 (2006), pp: 2305-2312  R. Ktinenkamp, R. Henninger, P. Hoyer “Photocarrier transport in colloidal titanium dioxide films”,J. Phys. Chem. 97 (1993), pp:7328-7330  Z. Qinnan, L. Baoshun, Z. Xiujian, „Effect of ratio of Oxygen to argon and thermal treatment on the structure and hydrophilicity of TiO2 thin films coated on glass by DC reactive magnetron sputtering” Rare Met. Mater. Eng 32 (2003), pp: 339-343  M. Nakamura, M. Kobayashi, N. Kuzuya, T. Komatsu, T. Mochizuka, Hydrophilic property of SiO2/TiO2 double layer films"Thin Solid Films 502 (2006),pp: 121-124  T. Sumita, H. Otsuka, H. Kubota, M. Nagata, Y. Honda,R. Miyagwa, T. Tsurushima, T. Sadoh, “Ion-beam modification of TiO2 film to multilayered photocatalyst,” Nucl. Instr. And Meth. B 148 (1999), pp: 758-761  A. Bendavid, P.J. Martin, A. Jamting, H. Takikawa, “Structural and optical properties of titanium oxide thin films deposited by filtered arc deposition” Thin Solid Films 355 (1999),pp: 6-11  W. Y. Teoh, R. Amal, L. Madler, S. E. Pratsinis, “Flame sprayed visible light - active Fe- TiO2 for photomineralization of oxalic acid” Catalysis Today120 (2007), pp: 203-213.  K. Ubonchonlakate, L. Sikong, F. Saito, “Photocatalytic disinfection of P.aeruginosa bacterial Ag-doped TiO2 film”, Procedia Engineering32 (2012), pp: 656-662  E. Aubry, M.N. Ghazzal, V. Demange, N. Chaoui, D. Robert, A. Billard, “Poisoning prevention of TiO2 photocatalyst coatings sputtered on soda-lime glass by intercalation of SiNx diffusion barriers”. Surf. Coat. Technol. 201 (2007), pp: 7706-7712.  M. Arab Pour Yazdi, P. Briois, S. Georges, F. Lapostolle and A. Billard, “Structural and electrical characterisation of strontium zirconate proton conductor co-sputter deposited coatings” Ionics14, (2008), pp: 285-291.  Z.b. Zhang, C.Ch. Wang, R. Zakaria, J.Y. Ying, « Role of Particle Size in Nanocrystalline TiO2-Based Photocatalysts », J. Phys.Chem. B. 102 (1998), pp: 10871-10878.  C.Y. Wang, D.W. Bahnemann, J.K. Dohrmann, « A novel preparation of iron-doped TiO2 nanoparticles with enhanced photocatalytic activity », Chem.Commun. (2000), pp: 1539-1540.  Y.Liu, C.Liu, Q.Rong, Z.Zhang, « Characteristics of the silver-doped TiO2 nanoparticles » Applied Surface Science. 220 (2003),pp: 7-11.  L.E. Depero, A. Marino, E. Bontempi, L. Sangaletti, C.Casale, M. Notaro, « Morphology and microstructural properties of TiO2 nanopowders doped with trivalent Al and Ga cations », J. Mater. Res. 15 (2000),pp: 2080-2086.  A. Hagfeldt, M. Gra¨tzel, « Light-Induced Redox Reactions in Nanocrystalline Systems », Chem. Rev. 95 (1995),pp: 49-68.  C. He, Y. Yu, X. Hu, A. Larbot, « Influence of silver doping on the photocatalytic activity of titania films », Applied Surface Science. 200 (2002),pp: 239-247.  H. Wang, J. Niu, X. Long, Y. He, « Sonophotocatalytic degradation of methyl orange by nano-sized Ag/TiO2 particles in aqueous solutions», Ultrasonics Sonochemistry. 15 (2008), pp:386-392.  H.M. Sung-Suh, J.R. Choi, H.J. Hah, S.M.Koo,Y. Chan Bae, “Comparison of Ag deposition effects on the photocatalytic activity of nanoparticulate TiO2 under visible and UV light irradiation” J. Photochem. Photobiol. A Chem. 163 (2004), pp:37-44.  G. Lassaletta, A.R. Gonzales-Elipe, A. Justo, A. Fernandez, F.J. Ager,M.A. Respaldiza, J.G. Soares, M.F. Da Silva, “ Thermal and photochemical methods for the preparation of thin films of cermet materials” J. Mater. Sci. 31 (1996), pp:2325-2332.